# mechanisms of diffusion in materials - mit .self-diffusion of solute atoms via vacancy mechanism

Post on 11-Jun-2018

212 views

Embed Size (px)

TRANSCRIPT

3.205 L4 11/7/06

Mechanisms of Diffusion in Materials

1

A final point on interdiffusion The composition profiles resulting from inter-

diffusion are generally constrained by phase equilibria. Consider the an IrRe diffusion couple annealed at 2400C:

Equilibrium diagram Diffusion couple

23.205 L4 11/7/06

Now consider the OsW system at 2200C :

In this case, a couple initially between pure Os and pure W can form an intermediate phase, , in the interdiffusion zone. If forms, the resulting composition curve will have two discontinuities.

33.205 L4 11/7/06

Illustration of interphase layer growth in XY alloy interdiffusion

Video clip from Diffusion in solid metalmultiphase system, V. Ruth (Universitt Oldenburg), K. Schaar, J. Thienel, and H.G. Graske (Institut fr de Wissenschaftlichen, Gttingen) IWF, Gottingen 1986

43.205 L4 11/7/06

Atomistic mechanisms for diffusion in crystals

Given sufficient thermal energy, an atom can

move from one site to another in a crystal.

Most diffusion in crystals occurs by either the vacancy mechanism or the interstitial mechanism.

53.205 L4 11/7/06

Figures removed due to copyright restrictions.See Figures 8.2 and 8.7 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter.Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891.

Atomistic mechanisms, contd

Additional mechanisms include the interstitialcy mechanism in crystals containing significant numbers of self-interstitials (e.g., produced by irradiation); and the reptation mechanism in molten (hence non-crystalline) polymers.

Interstialcy Reptation 63.205 L4 11/7/06

Atomistic mechanisms, contd Jumps of vacancies and interstitials are thermally

activated, and jumps occur at a jump rate, ,

!

" # = $ exp %Gm kT( )[ ]

is an attempt frequency typically ~1013 s1; and Gm is the free energy of migration.

The total jump frequency, , is = z , where z is the coordination number (z = 12 in f.c.c.).

73.205 L4 11/7/06

Figure removed due to copyright restrictions.See Figure 7.2 in Balluffi, Robert W., Samuel M. Allen, and W. Craig Carter.Kinetics of Materials. Hoboken, NJ: J. Wiley & Sons, 2005. ISBN: 0471246891.

Diffusion and random walks

During self-diffusion, vacancies and interstitials execute a random walk among sites in the crystal structure: the trajectories they follow involve a series of discrete jumps, and each jump is uncorrelated with the previous jump.

Illustrate the effects of a vacancy executing a random walk in a diffusion couple via Java applet

83.205 L4 11/7/06

Diffusion & random walks, contd

Mean-square displacement from a random walk of

n jumps each of length r:

!

R2 = nr2

and for a random-walking vacancy or interstitial, the self-diffusivity in three-dimensional systems is given by:

!

D ="r2

6

93.205 L4 11/7/06

Diffusion & random walks, contd

Diffusion in alloys: intrinsic diffusivity and

interdiffusivity

These can involve correlated jumps and the resulting value of the mean square displacement can be either greater than, or less than, that for self-diffusion. The correlation factor, f, accounts for the extent of correlation, with f = 1 for uncorrelated jumps:

!

R2 = nr2 " f and D =

#r2

6f

103.205 L4 11/7/06

Self-diffusion of interstitials

Involves only random walk of the interstitial species, and thus

!

DI ="I r

2

6f =

z # " I r2

6f =

z$r2

6exp %GI

mkT( )[ ] &1

=z$r2

6exp SI

mk[ ] & exp %HIm kT( )[ ]

Note that interstitial motion is uncorrelated, so f = 1.

113.205 L4 11/7/06

Self-diffusion of vacancies

Involves only random walk of vacancies, and thus

!

DV ="Vr

2

6f =

z # " Vr2

6f =

z$r2

6exp %GV

mkT( )[ ] &1

=z$r2

6exp SV

mk[ ] & exp %HVm kT( )[ ]

Note that vacancy motion is uncorrelated, so f = 1.

123.205 L4 11/7/06

Self-diffusion of solute atoms via vacancy mechanism

Involves exchange of randomly walking vacancies with the solute atom, A, and thus the atom jump frequency must relate to both the vacancy jump frequency and the probability that a site adjacent to the solute atom is vacant, XV. XV is equal to the equilbrium fraction of vacant sites,

!

XV = exp "GVf

kT( )[ ] = exp SVf k[ ]exp "HVf kT( )[ ]

133.205 L4 11/7/06

Self-diffusion of solute atoms via vacancy mechanism, contd

Using equations for D and

!

DA =Xvz"vr

2

6f =

zr2#

6exp $ GV

f +GVm( ) kT( )[ ] f

=zr2#

6exp SV

f + SVm( ) k[ ]exp $ HVf +HVm( ) kT( )[ ] f!

"A = XV"V = XV z # " V

The correlation factor, f, for vacancy diffusion in metals is about 0.7 and can be calculated more precisely for various specific cases.

143.205 L4 11/7/06